Board level failure analysis of chip scale package drop test
Board Level Failure Analysis of Chip Scale Package Drop Test Assemblies
Nicholas Vickers, Kyle Rauen, Andrew Farris, Jianbiao Pan
Cal Poly State University
San Luis Obispo, CA 93407
Email: email@example.com, firstname.lastname@example.org, email@example.com, firstname.lastname@example.org
This paper presents the failure analysis results of board level drop tests. In this study, the test vehicle was designed
according to the requirements of the Joint Electron Device Engineering Council (JEDEC) drop test board. The test
vehicle was assembled with 15 chip scale packages (CSPs) each having 228 daisy-chained 0.5 mm pitch solder
joints using Sn-3.0 wt% Ag- 0.5 wt% Cu (SAC305) lead free solder. Assemblies were drop tested using three
different peak accelerations of 900 G, 1500 G, 2900 G, with 0.7 ms, 0.5 ms, and 0.3 ms pulse durations,
respectively. Scanning electron microscopy (SEM) with energy dispersive spectroscopy and dye-penetrant methods
were applied to investigate the failure locations and the failure modes. The failure modes and solder joint locations
were mapped. Failure analysis showed that pad cratering was the most common failure mode and that this led to
trace cracking on the board side. Trace cracking was the second most common failure mode. Solder joint cracking
was also observed on the board side near the intermetallic layer, which was the third most common failure mode.
The results imply that the solder joint is more reliable than the printed circuit board during drop test.
Keywords: Lead free solder, drop impact test, pad cratering, failure analysis.
Ten trillion solder interconnections are made
annually in the electronics industry for mobile
devices, computers, and other communications,
medical, aerospace, and military applications . The
solder interconnection is the primary interconnection
in microelectronics packaging because it provides the
mechanical and electrical interconnection between
the package and the printed circuit board (PCB). If
one interconnection fails in a PCB, the whole board
and even the whole system may fail. Therefore,
establishing and improving the reliability of solder
interconnections is vital to the $1.3 trillion
Handheld consumer electronic devices are
prone to be dropped. The drop event may result in the
solder interconnection failure. The drop impact
response and failure characteristics are important
topics to understand in order to improve electronic
With the enactment and
enforcement of the European Union’s Restriction of
Hazardous Substances (RoHS) and similar legislation
around the world, the focus of reliability researchers
quickly shifted toward lead-free solder alloys. Tinsilver-copper (SnAgCu) is now a commonly used
lead-free solder alloy in the electronics industry.
The drop reliability of SnAgCu solder joints
has been researched by many [2-12]. Poor drop test
reliability of lead-free solders has been reported ,
because SnAgCu alloys have higher strength and
modulus than SnPb. Two ways to improve drop
testing reliability of SAC alloys are: lower Ag
content , and adding micro alloying . Both
methods result in many SAC alloys. However, the
failure mechanisms of drop test remain unclear.
The purpose of this research is to study the
failure mechanisms for board level lead-free chip
scale packages (CSPs). The final goal is to improve
the reliability of solder interconnections in
electronics assemblies through an improved
understanding of failure.
The test vehicle used was a JEDEC JESDB111 standard eight-layer FR4 test board as shown in
Figure 1. Fifteen chip scale packages (CSPs) were
attached to the test vehicle using a lead-free surface
mount assembly process. Each 12 mm square CSP
had 228 Sn-3.0 wt% Ag- 0.5 wt% Cu (SAC305)
solder joints at a 0.5 mm pitch that form an electrical
and mechanical connection to the circuit board. The
full details of the board assembly, drop testing
method, and reliability results are reported elsewhere
. The boards were drop tested using a Lansmont
MTS II shock test system and were dropped until a
majority of the CSPs experienced electrical failure.
Three different peak acceleration inputs were used in
drop testing: 900 G, 1500 G, 2900 G, with 0.7 ms,
0.5 ms, and 0.3 ms pulse durations, respectively. The
electrical continuity of each daisy-chained CSP was
verified before drop testing.
summarizes the percentage of each failure mode on
these 60 components analyzed. It shows that pad
cratering is the dominant failure mode for these test
vehicles in drop impact; 83.3% of the components
exhibited pad cratering. Pad cratering is defined as
cracking in the thin resin rich region underneath the
copper pads and traces as shown in Figure 3. Note
that some components had multiple failure modes so
that the total percentage shown in Figure 2 is more
Figure 1. Test vehicle assembly
Two failure analysis methods were used to
investigate the failure locations and the failure
modes: 1) dye-penetrant and 2) cross-sectioning
Scanning Electron Microscopy (SEM) with Energy
Dispersive Spectroscopy (EDS). Dye penetrant is a
common failure analysis method to examine preexisting cracks in solder joints, especially for Ball
Grid Array (BGA) and CSP solder joints. The
process works as follows. The PCBs were submerged
into a thermal-curable dye so that the dye will
penetrate into the crack area. After the dye is cured,
the components were pulled off exposing the
preexisting cracks. The components and boards were
examined using metallographic microscopes.
Cross sectioning SEM with EDS is another
common failure analysis technique to investigate the
crack location and intermetallic composition in solder
joints. Sample preparation starts with cutting sections
out of the PCB using a diamond abrasive saw. The
CSP and board section are mounted in a clear epoxy,
then ground and polished to expose the solder joint
cross section. A succession of sand papers were used
with the grit size from 80, following by the number
240, 320, 600, and 4000. The samples were then fine
polished using 0.3 and 0.05 alumina slurries. The last
steps were etching then sputter coating with a very
thin layer of gold. Cross sectioned samples were
etched with a 1% nitol etchant to evaluate the
microstructure. Micro hardness tests were done on
both the solder and resin to compare strengths of the
materials. The tests used a vickers microhardness
indenter at 100 grams of force.
After analyzing 60 components on four
boards that were dye penetrated, five failure modes
have been identified: 1) pad cratering, 2) solder
cracking near the board side, 3) solder cracking near
the component side, 4) input/output (I/O) trace
fracture, and 5) daisy chain trace fracture. Figure 2
Figure 2. Summary of failure modes
Figure 3. Copper pad cratering with dyed board
fibers, 100X magnification
Drop test reliability data shows that the
component location plays a significant role and the
components along the board center tend to fail
earliest and most frequently . To investigate
whether failure mode differs at different component
locations, the failure modes and the component
locations were mapped and shown in Figures 4 - 7.
The failure maps in Figures 4 - 7 show all
the solder joint locations and failure modes observed
for four test boards. All four boards were drop tested
at 1500 G peak acceleration, but the drop count
varies for each. The fill color in each device interior
indicates the stage of failure: green is not failed, cyan
is transitional failure (minor resistance change),
orange is temporary discontinuity, red is permanent
The individual solder joints are
indicated in the array around each device with failure
mode: white squares are not failed, black squares
indicate pad crater, red squares indicate solder crack
near board side, and yellow squares indicate solder
crack near component side (only 1 is shown).
Figures 4 and 5 show boards with no edgebonding applied to the CSPs, and Figures 6 and 7
show boards with edge-bonding applied . In
Figures 5 and 6, pad cratering is shown to occur on
nearly every CSP after relatively few drop impacts,
and may exist before without electrical failure occurs.
In a few cases electrical failure occurred by trace
cracking without pad cratering or solder fracture.
It is clear that pad cratering occurred mainly
in the corners of the CSPs with the exceptions to
components 3, 8, and 13, where it often happened
along the edges. The majority of pad cratering
occurred on one side of the board (toward component
6), which indicates asymmetric strain distributions
along the board. A dynamic failure measurement
system was used with a cable attachment near
Figure 4. Failure mode map for not edge-bonded board after 10 drops at 1500 G.
Figure 5. Failure mode map for not edge-bonded board after 14 drops at 1500 G.
Figure 6. Failure mode map for edge-bonded board after 279 drops at 1500 G.
Figure 7. Failure mode map for edge-bonded board after 325 drops at 1500 G.
It should be pointed out that pad cratering
does not necessarily lead to electrical failure of solder
joints. Figure 8 shows the relationship between pad
cratering and electrical failure. It shows that 19.4% of
components that had pad cratering did not fail
electrically. The figure also indicates that most
components that electrically failed exhibit pad
cratering, but pad cratering occurred on some
components that were not yet failed; pad cratering
was observed in combination with other failure
The second most common failure mode is
I/O trace fracture as shown in Figure 9. All
components that exhibit I/O trace failures also exhibit
pad cratering. 72.2% of pad cratered components
exhibit I/O trace fracture implying that the two
failure modes are coupled. Similarly all daisy chain
trace fractured components exhibit pad cratering,
implying that daisy chain trace fracture is caused by
pad cratering. Conversely, solder cracking appears to
be independent of pad cratering. This is shown by
Figure 8 where 5.6% of electrical failures are caused
by solder cracking where pad cratering was not
observed. Cracking of the solder joints on the board
side and component side was observed in 33.3% and
1.3% of the components, respectively.
Combining the failure analysis with the
reliability study previously reported , we see that
pad cratering indirectly causes electrical failure. The
reasons for this are simple, when the resin cracks
under the solder joint, stress is then shifted on to the
electrical trace on the PCB. When this occurs the
trace can fracture as illustrated in Figure 10. These
trace fractures occur both at outside trace connections
where the input and output signals occur, and also in
traces that connect solder balls within the BGA.
Figure 11 compares the ratios of failure
modes. Input/output trace failures were attributed to
causing 77% of the electrical failures. Of that 77%,
19% were in conjunction with solder fracture. Solder
fracture accounts for 12% of the electrical failures
observed, and 11% of the electrical failures were
caused by the daisy chain trace fracturing.
Cross sectioning SEM showed three
different failure modes: 1) pad cratering, 2) daisy
chain trace fracture, and 3) solder fracture on the
board side. Pad cratering as shown in Figure 12 was
observed near the corners of the component. Resin
cracks that cause pad cratering never penetrated into
the weave region and occurred only in the resin rich
region above the fiber weave near copper pads and
Resin cracks exhibited brittle fracture
characteristics. Both daisy chain trace cracking and
solder cracking as shown in Figure 13 are less
Figure 9. I/O trace cracked away from solder joint,
Figure 10. Illustration of cracked trace caused by pad
Figure 11. Percentage of electrical failure attributed
to the different material failure modes
Figure 12. Resin cracks beneath copper pad.
Magnification is 500X
Figure 8. The relationship observed between pad
cratering and electrical failure
Figure 13. Solder crack near board side IMC shown
on the right side of the picture. On the left is
evidence of a daisy chain trace fracture on the board
side at 100X magnification.
samples, an investigation of the solder ball
microstructure and also the relative strength of the
solder material compared to the resin was performed.
The resulting microstructure of the solder ball as
shown in Figures 14a and 14b shows small dendritic
grain growth. The smaller grains strengthen the
solder material. Failures are consequently shifted to
the weaker material, the resin. Figure 15 shows the
microhardness test results. The solder material had an
average microhardness of 72 while the resin has a
microhardness of 33. The result indicates that the
solder is much stronger than the resin. This finding
verifies that the resin is the weakest link and suggests
that pad cratering should be the most common
Figure 14a. Image of solder ball microstructure at
Figure 14b. Image of solder ball microstructure at
Figure 15. Results of the microhardness testing
The failure modes of drop testing CSP packages
with SAC305 solder joints assembled on a JEDEC
standard test vehicle are reported. The following
conclusions can be drawn from this study:
1. Pad cratering is the primary material failure
2. The board material is the weakest link in the
electronic assembly, will fail first, and will cause
other failures such as trace cracking.
3. Trace cracking due to pad cracking is more
common than solder cracking, especially where
traces are connected to outer array solder joints
and run outward from the CSP.
4. Majority failures occur at the corners of the
packages implying that the corners of the
components experience the most strain and
This work was partly supported by
Flextronics and Henkel Technology. Special thanks
to Mr. Jasbir Bath, Mr. David Geiger, Mr. Dennis
Willie, and Dr. Dongkai Shangguan of Flextronics,
Dr. Brian J. Toleno and Mr. Dan Maslyk of Henkel
Technologies for valuable technical support and
guidance. Thanks also go out to Michael Krist,
Micah Denecour, and Ronald Sloat for their support
and help on this research project. The first author
gratefully acknowledges the financial support from
National Science Foundation through Cal Poly’s
honors program and Surface Mount Technology
Association (SMTA) Silicon Valley Chapter to work
on this project.
 N. Brathwaite, “Forword,” Lead-free Solder
Interconnect Reliability, edited by D.
Shangguan, ASM International, p. vii, 2005.
 Y. Liu, G. Tian, R.W. Johnson, and L. Crane,
“Lead-free chip scale packages: assembly and
drop test reliability”, IEEE Transactions on
Electronics Packaging Manufacturing, Vol. 29,
No. 1, Jan. 2006, pp. 1-9.
 P. Marjamaki, T. Mattila, J. Kivilahti, “Finite
element analysis of lead-free drop test boards”,
Proceedings of 2005 IEEE Electronics
Components and Technology Conference, pp.
 M.A. Matin, W.P. Vellinga, M.G.D. Geers, ,
“Microstructural Stability and Failure Modes in
Eutectic Sn-Ag-Cu Solder”, 5th International
Conference on Thermal and Mechanical
Simulation and Experiments in Micro-electronics
and Micro-Systems, pp. 337-340.
 A.R. Zbrzezny, P. Snugovsky, T. Lindsay, and
R. Lau, “Reliability Investigation of Mixed BGA
Assemblies”, IEEE Transactions on Electronics
Packaging Manufacturing, Vol. 29, No. 3, pp.
 H. Lou, X. Qu, Z. Chen, J. Wang, T. Lee, and H.
Wang, “Lifetime assessment of solder joints of
BGA package in board level drop test”, Proc. of
IEEE 6th International Conf. on Electronic
Packaging Technology, 2005, pp. 696-700.
 F.X. Che, J.H.L. Pang, W.H. Zhu, W. Sun, A.
Sun, C.K. Wang, H.B. Tan, “Comprehensive
modeling of stress-strain behavior for lead-free
solder joints under board-level drop impact
loading conditions”, Proceedings of 2007 IEEE
ECTC, pp. 528-534.
 E.H. Wong, R. Rajoo, Y.M. Mai, S.K.W. Seah,
K.T. Tsai, and L.M. Yap, “Drop Impact:
Fundamentals & Impact Characterization of
Solder Joints,” Proceedings of 2005 IEEE
ECTC, pp. 1202 – 1208.
 D.Y.R. Chong, F.X Che, J.H.L. Pang, L. Xu,
B.S. Xiong, H.J. Toh, and B.K. Lim, “Evaluation
of influencing factors of board-level drop
reliability for chip scale packages (fine-pitch ball
grid array)”, IEEE Transactions on Advanced
Packaging, Vol. 31, No. 1, pp. 66-75, 2007.
 Y.S. Lai, P.F. Yang, and C.L. Yeh,
“Experimental studies of board-level reliability
of chip-scale packages subjected to JEDEC drop
test condition”, Microelectronics Reliability,
Vol. 46, No. 2, 2006, pp. 645-650.
 A. Farris, J. Pan, A. Liddicoat, B. J. Toleno, D.
Maslyk, D. Shangguan, J. Bath, D. Willie, D.
Geiger, “Drop Test Reliability of Lead-Free
Chip Scale Packages”, Proceedings of 2008
IEEE Electronics Components and Technology
Conference, pp. 1173-1180.
 D.Y.R. Chong, K. Ng, J.Y.N. Tan, P.T.H. Low,
J.H.L. Pang, F.X. Che, B.S. Xiong, L.H. Xu,
“Drop impact reliability testing for lead-free &
leaded soldered IC packages”, Proceedings of
2005 IEEE Electronics Components and
Technology Conference, pp. 622-629.
 H. Kim, M. Zhang, C.M. Kumar, D. Suh, P. Liu,
D. Kim, M. Xie, and Z. Wang, “Improved drop
reliability performance with lead free solders of
low Ag content and their failure modes”,
Proceedings of 2007 IEEE Electronics
Components and Technology Conference, pp.
 R.S. Pandher, B.G. Lewis, R. Vangaveti, and B.
Singh, “Drop shock reliability of lead-free alloys
-- Effect of micro-additives”, Proceedings of
2007 IEEE Electronics Components and
Technology Conference, pp. 669-676.